Metallic, Magnetic and Molecular Nanocontacts
Scanning tunnelling microscopy and break-junction experiments realize metallic and molecular nanocontacts that act as ideal one-dimensional channels between macroscopic electrodes. Emergent nanoscale phenomena typical of these systems encompass structural, mechanical, electronic, transport, and magnetic properties. This Review focuses on the theoretical explanation of some of these properties obtained with the help of first-principles methods. By tracing parallel theoretical and experimental developments from the discovery of nanowire formation and conductance quantization in gold nanowires to recent observations of emergent magnetism and Kondo correlations, we exemplify the main concepts and ingredients needed to bring together ab initio calculations and physical observations. It can be anticipated that diode, sensor, spin-valve and spin-filter functionalities relevant for spintronics and molecular electronics applications will benefit from the physical understanding thus obtained.
A nanocontact is a local point of contact between two macroscopic conductors where electrical current is constrained to pass through a cross-section about a nanometre wide. The conductance through a nanocontact is characteristically determined by the scattering on the local atomic and electronic structure of this region. Nanocontacts may consist of a single molecule, a constriction in a metallic wire, or even a monatomic chain of atoms, down to a single atom,agrait2003 and have been fabricated in break junctions,muller1992 scanning tunnelling microscopes (STMs),gimzewski1987 transmission electron microscopesohnishi1998 ; rodrigues2001 and on insulating substrates by electromigrationpark1999 and electrodeposition.li1999 ; morpurgo1999 With modern techniques it is possible to form molecular nanocontacts which are stable for several hours and can be mechanically controlled within a break junction or by an STM tip and electrically modulated by gate and bias voltages or the immediate nanoscale environment.
Gold nanocontacts are known for the remarkable phenomenon of conductance quantization,agrait1993 ; pascual1993 ; brandbyge1995 ; gai1996 ; ohnishi1998 ; yanson1998 which also occurs in some other metalskrans1993 ; olesen1994 and is one of the few quantum effects visible at room temperature. The famous ductility of gold extends to the nanoscale, where it readily forms stable monatomic wires with conductance quantized in units of , where is the elementary charge and is Planck’s constant. The conductance of transition metals is more complicated, but like that of gold can still be understood within the Landauer-Büttiker theory of ballistic conductance.landauer1957 ; buettiker1988 ; imry1999 Spontaneous magnetism, such as that predicteddelin2004b ; smogunov2008a ; smogunov2008b and observed strigl2015 in platinum nanocontacts, is a prime example of “small is different,”landman1992 that is, how nanoscale systems in reduced dimensions can behave differently than expected from what we know about their bulk material properties. With growing interest in nanocontacts from the fields of molecular electronicsaviram1974 ; joachim2000 ; tao2006 ; heath2009 ; scott2010 and spintronics,zutic2004 ; sanvito2011 investigations have recently broadened to molecular nanocontacts, which present additional electronic, spin and vibrational complexities, as well as many-body phenomena, such as Coulomb blockade and the Kondo effect.
The purpose of this focused Review, with no claims of completeness, is to summarize an arc of interrelated developments stretching from foundational work on gold nanowires and conductance quantization to magnetic nanocontacts and finally dynamical magnetic correlations in the form of Kondo conductance anomalies. Emphasis is placed on the intersection of state-of-the-art first principles electronic structure calculations and experiment in the decade following a review of metallic point contacts.agrait2003 In view of the recent experimental verification of several theoretical predictions, it is now an ideal time to summarize anew the status of the field. The topics covered include the structure and mechanics of metallic nanocontacts, ab initio-based ballistic electron transport as described by the Landauer-Büttiker scattering formalism, magnetic nanocontacts with separate spin-up and spin-down conductance channels, noise measurements for identifying spontaneous emergent magnetism, Kondo conductance anomalies in transport through transition metal adatoms and molecules, and exotic Kondo physics involving a breakdown of the Fermi liquid picture. Magnetic and molecular nanocontacts are of particular interest for their potential device applications as discussed in the final section.
Mechanics and structural properties
Accidental nanocontacts routinely form and break in the context of friction between bodies. Specifically planned nanocontacts may be fabricated by a variety of techniques. In break-junction experiments, it was found that a notched wire under tension develops a narrow neck before eventually breaking. Bringing the ends back together forms a point contact, sometimes with the cross-section of a single atom. In STMs, a sharp metal tip is pushed into a metallic surface and gradually retracted until the contact has shrunk to a single atom. Just before the breaking point, the conductance of these nanocontact systems decreases in approximately quantized steps. The closeness of the very last steps to multiples of indicates that the last contact is a single atom wide. All this early work has been superbly reviewed by Agraït and colleagues.agrait2003 Experimental work has been paralleled by numerical simulations,landman1990 ; sutton1990 ; guelseren1998 ; nakamura1999 ; hakkinen2000 ; bahn2001 ; dasilva2004 ; coura2004 ; dednam2015 usually of the molecular dynamics type, where interatomic forces are provided by one or another force field. Since simulations can only handle extremely short times, it is important to address the general issue of timescales.
Conceptually, the process of breaking a ductile metallic nanocontact under traction involves a multiplicity of timescales. The first and shortest, , is that of initial plastic yield, slippage, atom rearrangement, and a very system-specific local thinning with destruction of the bulk crystalline structure. On a second, longer timescale, , a slower flow of atoms may, if ductility is sufficient, establish a nearly steady state between the bulk-like “leads” and the nanocontact region. As we shall see below, in ductile metals such as gold, platinum, and some alkalis, the nanocontact may adopt well-defined, long-lived even if temporary, near-equilibrium geometrical shapes, such as nanowires. The nanocontact is in this case under an effective tension (even in the absence of traction) which drives an associated flow of atoms away from the contact and into the bulk-like leads. During this spontaneous thinning process, the nanocontact evolves through thinner and thinner shapes, lingering for longer times in those whose “magic” structures are energetically favourable. Alternatively, in less interesting non-ductile materials, there is no time to attain this metastable stage before the third timescale, , is reached, where the nanocontact snaps and breaks. Time scale may be realistically reached and atomistically described in real time by molecular dynamics simulations. The longer timescale is instead generally beyond reach.
As an alternative to simulations, the process of adiabatic nanocontact thinning can be given a thermodynamic description, which is revealing even if approximate. Let us discuss here the case of nanowires. A phenomenon that attracted attention is the spontaneous appearance during pulling, particularly in gold, of metallic wires with quantized diameters and shapes, reaching a length of several nanometres before breaking. Physical reasons behind the formation of nanowires were given in Ref. tosatti2005, , following earlier proposals,torres1999 ; tosatti2001 as well as in Ref. hakkinen2000, .
Simulations had predictedguelseren1998 that free nanowires could adopt “weird” non-crystalline helical shapes below a critical radius. A spectacular variety of magic (meaning reproducibly well-defined) weird nanowire shapes were discovered by Takayanagi’s group in their transmission electron microscopy study of gold nanocontacts suspended between leadskondo2000 (see Fig. 1a-d).
Predicting the actual magic shapes observed in this geometry turns out to require not just the ab initio effort to calculate the total energy (where is the number of atoms in the wire) as a function of shape, but also the thermodynamic consideration that a suspended nanowire is free to exchange atoms with the leads, actually bringing it into grand canonical equilibrium with them. The resulting equilibrium configurations are determined by the minima of
where is the chemical potential of an atom in the bulk-like metal leads, and is the nanowire length.tosatti2001 An atom in a nanowire always has a higher energy than in the infinite bulk, making positive definite. With the dimensions of force, represents the thermodynamic string tension of the suspended nanowire, whose minimum is only attained for . The adiabatic shape evolution of a suspended nanowire in time is governed by the progressive and spontaneous decrease of , sketched in Fig. 1e, actuated by jump-like drops in and therefore in radius, until the nanowire finally breaks when . As it turns out, the magic nanowire structures are helical (Fig. 1f versus Fig. 1g,h) because for the same number of atoms a helical twist reduces the radius and increases the length , therefore lowering the nanowire string tension, very much as would happen in a rolled up sheet of paper. Short monatomic chains of gold—the minimal nanowires—were also found and recorded in stunning real-time transmission electron microscope movies.ohnishi1998 Break junction data clearly identified them in gold and also platinum.yanson1998 ; smit2001 The simple string tension model works qualitatively in this case too.tosatti2005
It should be noted that the microscopic mechanisms leading to the energy minimizing structure of magic nanowires may be of different types. In noble, transition and other metals where cohesion involves a multiplicity of electronic contributions, minimal energy configurations are generally believed to correspond to optimal packing of the atoms.guelseren1998 In alkali metals, where nanowires were observed in break-junction work,yanson2001 the energy minima may also be determined by electronic shell closing.urban2004
Nanocontacts operate in the ballistic, as opposed to diffusive, transport regime when the elastic mean free path is much greater than the characteristic dimension of the contact. Quantum effects come into play when is small enough to be comparable to the Fermi wavelength . Nanocontacts meet this requirement, as is on the order of 5Å in metals. A contact region of width is expected to support only a finite number of conducting channels due to wave quantization in the transverse direction, analogous to waveguides.
Landauer-Büttiker formalism is a linear response theory that describes quantum ballistic transport in terms of the transmission and reflection coefficients of conduction electrons scattering off the contact region.landauer1957 ; buettiker1988 ; imry1999 A typical scattering geometry is represented in Fig. 2.
The number of conducting channels at a given energy in the left and right leads, and , is determined by the number of bands crossing that energy. The amplitudes of incoming and outgoing channels are related by the scattering matrix
where is the matrix containing the transmission amplitudes connecting each of the incoming channels of the left lead with each of the outgoing channels of the right lead and is the matrix of reflection amplitudes. Similarly, and describe transmission and reflection of states incident from the right lead. When the chemical potentials in the left and right leads are fixed to and , the current through the nanocontact is given by the Landauer-Büttiker formula
Here, the energy-dependent transmission function is the trace of the product of and its hermitian conjugate , and is the Fermi-Dirac distribution function. At zero temperature, the Landauer-Büttiker formula implies the differential conductance at zero bias voltage ():
where the summation is over the eigenchannel transmission probabilities (eigenvalues of ) and is the spin index. This remarkably simple formula depends only on the universal conductance quantum and the transmission function at the Fermi energy . In non-magnetic nanocontacts, one often redefines the conductance quantum as by summing over spin independent in Eq. (4), but we will not do so here. Quantum ballistic conductance depends on details of the quantum mechanical scattering off the contact region and is therefore a consequence of the wave nature of electrons. Equations (3) and (4) in fact assume that the wavefunction maintains phase coherence throughout the nanocontact region, and Eq. (3) is adequate only for sufficiently low bias voltage, as the Landauer-Büttiker theory is based on linear response.
Conductance quantization,agrait1993 ; pascual1993 ; krans1993 ; olesen1994 ; brandbyge1995 ; gai1996 ; ohnishi1998 ; yanson1998 as plotted for an STM nanocontact in Fig. 3a, is a remarkable property of quantum ballistic transport.
Similar behaviour is observed in break-junction experiments. The last plateau is particularly flat and well defined and occurs close to . In some metals, the last plateau persists despite an elongation much greater than the interatomic spacing. This indicates that the single atom contact progressively lengthens into a chain of up to 10 atoms as the tip is retracted.yanson1998 ; ohnishi1998 ; kizuka2008 Chain formation is favoured in 5 metals, such as Ir, Pt, and Au, over 4 metals due to multi-atom forces,ercolessi1988 ; tosatti2005 ultimately rooted in relativistic effects.takeuchi1989 ; agrait2003 Real-time images of the structure and mechanics of chain formation have been acquired in transmission electron microscopes.ohnishi1998 ; rodrigues2001 ; kizuka2008 ; lacroix2014 Since the width of the chain is a single atom, only one broad -like conduction band is open and contributes per spin, while all other bands have . For other metals, particularly transition metals with partially filled bands, the lowest plateau often occurs at a conductance greater than . An upper limit is set by the chemical valence of the bridging atom.scheer1998
The atomic-scale variability of the nanocontacts causes a degree of randomness in the positions of the conductance plateaus, but after several repetitions of the experiment a preference for certain values can be discerned. To analyse this trend systematically, large data sets of individual conductance versus displacement curves are collected and plotted as histograms. Figure 3b shows an example of a histogram for Au nanocontacts at room temperature.brandbyge1995 Similar histograms are obtained for other noble metals (Cu, Ag) and the alkali metals (Li, Na, K). Ab initio calculations for short Au chains suspended between bulk leadsbrandbyge2002 ; palacios2002 ; mehrez2002 reproduce well the experimental conductance 2 of the last plateau.
Although many of the lowest conductance plateaus occur close to integer multiples of , it is not straightforward to interpret them as evidence of conductance quantization of the type found in two-dimensional electron gas point contacts,vanwees1988 ; wharam1988 where the conductance jumps sharply but continuously by as the width of the contact is varied, because the cross-section of a nanocontact cannot be varied continuously, due to the atomic granularity.agrait2003 From simultaneous measurements of the conductance and force on the STM tip,rubio1996 ; rubiobollinger2001 as well as analogous molecular dynamics simulations,todorov1996 ; sorensen1998 the sharp jumps in the conductance have been correlated with abrupt atomic-scale rearrangements of the nanocontact geometry. The height of the conductance steps is not always quantized to an integer multiple of , and their position varies from trace to trace and from metal to metal. Thus, it is not always straightforward to attribute them to the opening or closing of individual channels with close to 1.
The key input of the Landauer-Büttiker formula is the scattering matrix , but the formalism itself does not provide a prescription for modelling the nanocontact geometry or calculating its matrix. Many different approaches have been developed for that purpose (see Refs. brandbyge2002, ; palacios2002, ; calzolari2004, and references therein). Here we review an ab initio method for solving the quantum mechanical scattering problem for realistic nanocontacts,smogunov2004a based on the complex band structure approach.choi1999 An implementation of the method is available in the electronic structure code Quantum Espresso.giannozzi2009
The self-consistent Kohn-Sham potential from a ground-state density functional theory (DFT) calculation of the scattering region and left and right leads, as illustrated in Fig. 2, provides the potential defining the quantum mechanical scattering problem. The asymptotic form for the scattering state of the th incoming Bloch wave of the left electrode as is
The wavefunction in the scattering region is matched to the wavefunctions in the leads by requiring continuity of and at the matching planes shown in Fig. 2. To achieve a smooth matching, it is crucial that the wavefunction in the left lead is expanded not only over the propagating Bloch waves with real crystal momentum but also over generalized Bloch states with complex , which decay to the left. Analogous considerations apply to the right lead. Inside the scattering region, where the translational symmetry is broken in the direction, the Schrödinger equation is solved numerically on a dense sequence of planar slices.
This approach delivers the full matrix and the scattering phase shifts , defined from the eigenvalues of , diagonalized by a unitary matrix , i.e.
The scattering phase shifts, which depend on the energy of the incoming wave, can be used to calculate several relevant quantities, such as the orbital-resolved density of states of a given scattering eigenchannel. The approach includes full spin-orbit interactions, noncollinear magnetism and, if relevant, corrections to the nanocontact electronic structure due to the Hubbard repulsion and exchange coupling of localized orbitals. Any atomistic model can be used for the leads and scattering region, which are treated on equal footing. Inelastic vibrational or magnetic excitations and non-equilibrium effects are not directly included.
In nanocontacts with ferromagnetic leads, one might expect conductance quantization in units of (instead of ), if spin degeneracy is lifted. This is not what is observeduntiedt2004 because in magnetic nanocontacts there are typically several partially open channels which generally add up to give non-integer . Moreover, there is no peak at , as the occurrence of magnetism in the bands does not shut off the -like minority spin channel,smogunov2004a except in the presence of impurities.untiedt2004
Histograms of STM conductance measurements show that Ni has broad peaks at 2.6-3.2 and 6 (Refs. sirvent1996, ; oshima1998, ; ono1999, ; bakker2002, ; untiedt2004, ), Co has broad peaks at 2.5 and 5 (Ref. untiedt2004, ) and Fe has a broad peak at 3.6-4.4 (Refs. ludoph2000, ; untiedt2004, ). The conductance of the lowest peak (the last plateau before breaking) is thus much smaller than the upper bound of based on the valency of the contact atom. Although the transmittance of light-mass channels remains close to 1, that of heavy-mass channels is much smaller. Despite this complexity, in addition to that associated with uncertainties in the structure and magnetic state of the contact, it has nevertheless proved possible to achieve semi-quantitative agreement between ab initio conductance calculations and experiment for a wide range of metals.
Ab initio calculations for a Ni nanocontact formed by two end-on (001) pyramid-shaped leads whose vertex atoms are 2.6 Å apart found a conductance of 3.85; the minority spin channel contributed 2.8 and the majority spin channel 1.05 (Ref. jacob2005, ). Calculations for a three-atom Ni chain suspended between bulk (001) electrodes using the ab initio Landauer-Büttiker approach described in the previous section obtained , of which comes from the minority spin channel and 1.0 from the majority channel.smogunov2006 The conductance of linear and zigzag three-atom Co chains between (001) Co leads was calculated to be -, depending on the geometry and magnetic configuration.bagrets2004
The magnetization of the left and right ferromagnetic leads is not necessarily aligned in experiment. In calculations of an ideal monatomic Ni nanowire, the presence of a magnetic domain wall, that is, antiparallel magnetization of the two leads, has been shown to completely block the channels, lowering the conductance from the ideal value of 7 to 2.smogunov2002 ; smogunov2004a ; smogunov2004b This results in very high values of magnetoresistance, MR, where and are the conductances for parallel and anti-parallel magnetic alignments. For more realistic two-atom Ni nanocontact geometries, more moderate values of MR were theoretically reported,jacob2005 as a consequence of the much smaller conductance of the channels due to their strong contact back-scattering. Similarly, the MR of few-atom chains of Co, Cu, Al and Si suspended between Co leads was found to be below 50% in all cases investigated.bagrets2004 Another important property is the anisotropic magnetoresistance, which reflects the dependence of the conductance on the relative angle between the electric current and the magnetization direction. This phenomenon was reported in the ballistic regime for Ni, Co, and Fe atomic-scale nanojunctions,autes2008 ; sokolov2007 following a theoretical prediction.velev2005
The degree of spin-polarisation of the current, defined as , where is the total spin- conductance, is restricted in magnetic transition metal nanocontacts by the fact that both spin-up and spin-down -like channels conduct almost perfectly. Therefore, the total current is only partially spin-polarized, e.g., values of about were reported in Ni nanocontacts.smogunov2006 A symmetry-based mechanism to fully block the spin-up conductance by joining two ferromagnetic electrodes with a special class of nonmagnetic -conjugated molecule has recently been proposed.smogunov2015 Molecules with only -symmetry orbitals around the Fermi level will reflect both spin-up and spin-down -symmetry channels coming from the ferromagnetic electrode. Only spin-down channels compatible with the molecular -orbitals will be allowed to pass through the junction, providing perfect spin-polarized conductance. A similar blocking mechanism was predicted to occur due to the -symmetry orbitals of oxygen impurities in Ni nanocontacts, leading to a MR of 700%.jacob2006
Magnetism was predicted to emerge spontaneously in reduced dimensions in the nominally non-magnetic metals platinumdelin2003 and palladium.gava2010 In DFT calculations, a Pt nanowire chain magnetizes parallel to the direction of the wire (easy axis magnetization) as a result of the narrowing of the bands and the cooperative effect of spin-orbit-coupling induced orbital magnetic moments.delin2003 ; delin2004b ; smogunov2008a ; smogunov2008b The ballistic conductance of a one-atom Pt contact suspended between (001) bulk leads was calculated to be 2.1,fernandezrossier2005 and for three-, four- and five-atom Pt chains it varies between 2.0 and 2.3,smogunov2008a in good agreement with break-junction experiments.krans1993 ; smit2001 ; smit2002 ; nielsen2003 The calculations have also revealed rather moderate values of ballistic anisotropic magnetoresistance, up to for the longest five-atom Pt nanocontacts.smogunov2008a Magnetism in Pt break-junction nanocontacts with approximately one- to four-atom chains has recently been confirmed by a gamut of experimental measurements.strigl2015
Shot noise and contact magnetism
Shot noise is a measure of non-equilibrium current fluctuations. While ballistic conductance is connected with the wavelike behaviour of electrons, shot noise depends on their particle nature through the discreteness of the electron charge. Assuming a Poissonian distribution of electron arrival times (tunnelling events), Schottky showed that the current noise power spectrum is approximately frequency independent and derived the classical relationship where is the average current. The current noise power spectrum is defined as
where and is the current in lead . In the low-temperature limit (where is the Boltzmann constant and is temperature) and with the help of approximations relevant for ballistic nanocontacts (see Ref. blanter2000, for a review), the noise power at a given lead simplifies to , where the Fano factor
describes the quantum mechanical suppression of Schottky’s classical result.
Since shot noise depends nonlinearly on the transmission probabilities , it represents an independent experimental probe providing information about the beyond that obtained from ballistic conductance measurements. The quantized conductance steps observed during the stretching of a Au nanocontact have been attributed to the spontaneous closing of channels with each successive atomic rearrangement of the local contact geometry. All are presumed to be either fully open or fully closed (1 or 0), except a single spin-degenerate channel carrying a fraction of a conductance quantum, i.e., . If this is the case, then according to Eq. (8) the shot noise should be suppressed when ; This suppression is indeed observed,vandenbrom1999 corroborating the standard interpretation. In other metals such as Al, the measured shot noise is not consistent with this scenario and can only be explained if multiple fractionally-open channels contribute to the conductance, vandenbrom1999 which agrees with the results of independent measurements on superconducting Al nanocontacts.scheer1997 Recent investigations of STM Au break junctions have found that also the ensemble variance of the shot noise is suppressed at (Ref. chen2014, ).
For a given value of the conductance , the shot noise has definite maximum and minimum values corresponding to different distributions of the . The upper bound is achieved by taking all . The lower bound occurs when all channels except one are either fully open or fully closed, as occurs in Au nanocontacts. Since the lower bound for magnetic states is below the lower bound of non-magnetic states, shot noise may be used as an experimental probe of nanocontact magnetism.kumar2013 ; burtzlaff2015 Simultaneous measurements of and for elongated Pt nanocontacts found a cluster of points all lying above the non-magnetic lower bound with a significant accumulation of points right at the boundary, as shown in Fig. 4.
While this at first suggests a non-magnetic state, ab initio ballistic transport calculations for the nanocontact geometry in Fig. 2 determined that the results are nevertheless consistent with a magnetic state, as the channels involved in conductance, and hence in shot noise, are weakly spin-polarized “spectators” of the magnetic state of the nanocontact, whereas the “actor” channels driving magnetism are very poorly conducting.kumar2013 Simultaneous and measurements have been used to estimate the spin polarisation of the conductance through Co and Fe adatoms on the Au(111) surface.burtzlaff2015
Kondo conductance anomalies
The nanocontact magnetism reviewed thus far has been static magnetism, a situation where, as in bulk magnets, the symmetry breaking mean-field picture of local magnetic moments aligned in a specific direction is valid and one can talk about separate spin-up and spin-down conductance channels. This picture breaks down if the magnetic moment of the contact region is small enough that it can flip through spin-flip scattering with conduction electrons on the experimentally relevant timescale, determined by the inverse width of the sharpest zero bias features in the I-V spectrum. In such situations the magnetism is dynamical.
In the simplest case of a spin- single atom nanocontact, spin-flip scattering “screens” the local magnetic moment, creating a many-body singlet state and restoring the spin symmetry which was broken in a static mean-field calculation. This is the Kondo effect in a nutshell.hewson1993 The screening is gradually suppressed as the temperature is raised above the characteristic Kondo temperature , which depends on the strength of the coupling with conduction electrons. Relatively difficult to detect experimentally in bulk materials, the Kondo effect is utterly relevant to transport in magnetic nanocontacts because the low-energy spin-flip scattering processes generate a resonance in the density of states at the Fermi energy, fundamentally altering low-bias transport. For typical experimentally measurable in the range of 1-100 K, the Kondo screening occurs on a short timescale s, meaning that transport experiments see the many-body singlet state and not the bare impurity spin. The Kondo effect has been observed in scanning tunnelling spectroscopy of Co adatoms on gold,madhavan1998 silver,wahl2004 and copperwahl2004 ; manoharan2000 ; neel2007 ; vitali2008 surfaces, Ce adatoms on silverli1998 and Fe and Co impurities beneath the copper surface,prueser2011 and in Fe, Co, and Ni break junctionscalvo2009 as a sharp zero-bias conductance anomaly with Fano lineshape.ujsaghy2000
The Kondo effect is also relevant for nanocontacts containing magnetic molecules,scott2010 for example, molecules containing transition metals or radicals with unpaired electrons. Essentially, the Kondo anomaly at the Fermi energy provides a transparent path at zero bias through molecules that would otherwise be insulating and totally reflecting. Zero-bias Kondo conductance anomalies have been reported in break-junction experiments with transition metal-bearing molecules,park2002 ; liang2002 ; parks2010 ; rakhmilevitch2014 molecules,yu2004 ; parks2007 ; roch2009 a long -conjugated chainosorio2007 and an organic radical,frisenda2015 and scanning tunnelling spectroscopy of adsorbed transition metal-bearing molecules,wahl2005 ; zhao2005 ; iancu2006 ; komeda2011 ; mugarza2011 ; minamitani2012 ; karan2015 a -conjugated molecule,temirov2008 and organic radicals.muellegger2013 ; zhang2013 ; requist2014
Figure 5 shows an example of a zero-bias anomaly and its temperature dependence for a spin- Kondo system.
Break junction-like nanocontacts containing a suspended molecule can also be created in an STM as illustrated in Fig. 6.
The molecule usually contains chemical linker groups that bond to metals, such as thiols, amines or pyridines. As in break junctions, the nanocontact can be mechanically controlled by varying the distance between the tip and surface.xu2003 ; quek2009 ; aradhya2013 Molecular contacts between an STM tip and surface have also been found to form spontaneouslyhaiss2003 or after an applied voltage pulse.sotthewes2014
The type of Kondo effect (fully screened, underscreened, singlet-triplet, two-stage, etc.) that occurs in a given nanocontact is totally determined by the nature of the conducting channels, which are in turn dependent on the local atomic positions and magnetic polarisation. In calculations, those details are generally decided on the basis of Anderson impurity model calculations with empirically chosen parameters – an approach which becomes increasingly difficult in multiorbital, multivalence situations and one which does not unambiguously determine the atomic or molecular orbitals involved. Ab initio calculations single out the relevant localized states and interactions but cannot be used to directly calculate zero-bias conductance anomalies since the static mean-field picture of spin-polarized DFT is not valid for dynamical magnetism and the common semi-local exchange-correlation functionals do not include Kondo correlations.
The ab initio ballistic scattering approach described above has been extendedlucignano2009 to treat Kondo conductance anomalies by linking DFT with the numerical renormalization group method (NRG),hewson1993 ; bulla2008 ; zitko2009 a many-body technique for calculating the Green’s function and thermodynamic properties of localized magnetic states in contact with conduction bands. The DFT+NRG method was originally used to calculate the Kondo conductance of an idealized Au nanowire with Ni impurity.lucignano2009 Calculations have also reproduced experimental trends in the Kondo temperature of a Co adatom on different Cu surfaces,baruselli2015 although discrepancies remain for the Fano lineshapes, which are sensitive to surface states and the atomic structure of the tip-adatom-surface contact. Being a parameter-free method, the DFT+NRG method has been used to predict Kondo conductance anomalies for impurities on carbon nanotubes.baruselli2012b The Kondo anomaly in the simplest molecular radical, nitric oxide, on the Au(111) surface was predicted in this way and subsequently confirmed by scanning tunnelling spectroscopy.requist2014 NRG calculations based on effective models have also been made for larger molecules.diasdasilva2009 ; cornaglia2010 Non-equilibrium effects, such as those occurring at finite bias, are potentially relevant in some situations but are not covered in this Review.
Although NRG is a numerically exact “gold standard,” it can only correlate two or three orbitals at a time due to computational limits. Other approaches to building many body correlations on top of mean-field DFT calculationsjacob2009 ; costi2009 ; surer2012 are able to approximately correlate the entire shell of a transition metal impurity. Calculations have been made for transition metals in metallic hostssurer2012 and large surface-adsorbed inorganic molecules, such as manganese phthalocyaninejacob2013 and manganese porphyrin.karan2015
Exotic Kondo effects
In the previous section we mainly discussed fully screened Kondo models, which show Fermi-liquid properties á la Noziéres;nozieres1974 in these systems a spin is screened by conduction channels, with . Models displaying non-Fermi-liquid behaviour include under- and over-screened Kondo models,nozieres1980 ; hewson1993 where, respectively, and ; when and , the problem is usually known as the two-channel Kondo effect. Even though these models are difficult to achieve in bulk magnetic alloys, where the metal hosts possess enough scattering channels to perfectly screen the magnetic impurity (), they can be realized in nanocontacts. For example, the underscreened Kondo effect has been observed for spin-1 Co complexesparks2010 and C moleculesroch2009 in break junctions.
One case which so far remains elusive is the ferromagnetic Kondo model,koller2005 where but the impurity and the conduction electrons are coupled ferromagnetically by an effective exchange interaction () rather than antiferromagnetically () in the Kondo exchange Hamiltonian with spin operators and for the conduction channel and impurity. The ferromagnetic Kondo effect will occur, for instance, when the impurity contains one level which is spin-polarized but totally uncoupled to the leads, and another level that couples to the leads but is only weakly spin polarized by intra-site Hund’s coupling. Although examples of this are at present only theoretical,koller2005 ; mehta2005 ; lucignano2009 the ferromagnetic Kondo model is important as the simplest example of non-Fermi liquid behaviour. At low temperature the impurity spin behaves essentially as a free local moment, apart from logarithmic singularities,koller2005 ; mehta2005 since a ferromagnetic coupling renormalizes to zero.anderson1970 Its spectral function displays a logarithmic “dimple” at and has peculiar temperature and magnetic-field dependence.baruselli2013 A finite temperature cuts off the logarithmic dimple at low frequency, while a magnetic field, no matter how small, destroys the logarithmic dimple replacing it with a symmetric pair of inelastic spin-flip Zeeman excitations.
Even though an experimental demonstration of the ferromagnetic Kondo effect is still lacking, a few proposals have been put forward, including transition metal impurities in the bulk of transition metals,gentile2009 substitutional Ni atoms in Au nanocontacts under strain,lucignano2009 and systems of multiple laterally coupled quantum dots. kuzmenko2006 ; baruselli2013 ; mitchell2013 ; andrade2015 In this last case, it is possible to induce a Berezinskii-Kosterlitz-Thouless transition through application of a gate potential or an additional interdot coupling.baruselli2013 ; mitchell2013 Ferromagnetic Kondo systems could in principle be realized with surface-adsorbed molecular radicals; however, up to now, only radicals with small, but still positive , have been observed.zhang2013
Representing the smallest foreseeable interface between nanoscale electronic devices and metallic electrodes, the nanocontacts reviewed here are likely to be an integral part of future electronic technologies. In molecular devices with metallic leads, it will be crucial to understand the electronic structure of the electrode-molecule bond. We now survey some specific technologically relevant applications involving nanocontacts.
After the seminal proposal of Aviram and Ratneraviram1974 envisioning a donor-acceptor molecule functioning as a diode, many other molecular devices have been proposed; for reviews of experimental progress, see e.g. Refs. joachim2000, ; tao2006, ; heath2009, . The conductance through molecular diodes, transistors and other devices can be calculated with the ab initio transport theories reviewed here.
Current rectification has been realized in several different molecular nanocontacts,metzger2003 ; elbing2005 ; diezperez2009 ; batra2013 where molecular orbital-electrode hybridisation is thought to crucially influence diode performance. Realising molecular transistors poses further challenges because they require a method of gating the source to drain current. Single-molecule break-junction devices have been gated from below via the substrate,park2000 ; park2002 ; liang2002 ; yu2004 ; roch2008 ; song2009 which proves the possibility of electrically gating molecular orbitals, even if not yet providing a scalable solution for molecular electronics. STM molecular nanocontacts are not conducive to electrical gating by a third terminal; however, the electrostatic potential of nearby charged adatoms can provide a gate potential.martinezblanco2015 Other ways to achieve gating have been proposed, including mechanical, chemical, optical, magnetic and electrochemical gates (see Ref. tao2006, and references therein). Mechanical compression of an STM bridge molecule has also been demonstrated to modulate conductance.quek2009 ; sotthewes2014
Computing devices that would make use of the electron spin attract interest for their advantages in terms of efficiency, storage density and the potential unification of memory and logic operations in the same device. We highlight here a few applications where ballistic conductance through magnetic and molecular nanocontacts may be of relevance to spintronics applications.
Memory devices such as magnetic random access memory and hard-disk read heads rely on the magnetoresistance of two ferromagnetic plates separated by a thin insulating layer. Attempts to scale down the basic memory unit by using atomic and molecular nanocontacts with high magnetoresistance, that is,“spin valve” behaviour, are being pursued. Generally, only modest values of magnetoresistance are obtained in metallic nanocontacts,bagrets2004 ; jacob2005 ; smogunov2008a although a larger value of has been calculated for a Au chain between Co electrodes, sivkov2014 a configuration which also realizes a relatively highly spin-polarized conductance due to the blocking of the minority spin channels by strong - hybridisation at the Co/Au interface. Larger values of magnetoresistance have been calculated and observed for molecular nanocontacts,pati2003 ; rocha2005 ; schmaus2011 ; tao2013 ; zu2013 ; smogunov2015 reaching (ideally) infinite magnetoresistance for certain non-magnetic -conjugated molecules between ferromagnetic leads.smogunov2015
Highly selective spin filters are sought for spintronics applications. As reviewed in the Magnetic Junctions section, it is difficult to achieve a fully spin-polarized current in purely metallic nanocontacts. An alternative is provided by transition metal oxides, particularly nickel oxide, which, as mentioned above, was predicted to become half metallic in reduced dimensionsjacob2006 and has recently shown evidence of nearly complete spin filtering when realized by oxygenation of nickel break junctions.vardimon2015 Several proposals for molecular spin filters have recently been put forward (see e.g. Refs. sanvito2011, ; zu2013, ; smogunov2015, and references therein), where spin-filtering behaviour is often connected with magnetoresistance. The molecular bonding group and its spin-dependent hybridisation with the leads is an important factor determining the performance of molecular spin valves and spin filters.
- (1) Agraït, N., Levi Yeyati, A. & van Ruitenbeek, J. M., Quantum properties of atomic-sized conductors. Phys. Rep. 377, 81 (2003).
- (2) Muller, C. J., van Ruitenbeek, J. M. & de Jongh, L. J., Conductance and Supercurrent Discontinuities in Atomic-Scale Metallic Constrictions of Variable Width. Phys. Rev. Lett. 69, 140 (1992).
- (3) Gimzewski, J. K. & Möller, R., Transition from the tunneling regime to point contact studied using scanning tunneling microscopy. Phys. Rev. B 36, 1284 (1987).
- (4) Ohnishi, H., Kondo, Y. & Takayanagi, K., Quantized conductance through individual rows of suspended gold atoms. Nature 395, 780 (1998).
- (5) Rodrigues, V. & Ugarte, D., Real-time imaging of atomistic process in one-atom-thick metal junctions. Phys. Rev. B 63, 073405 (2001).
- (6) Park, H., Lim, A. K. L., Alivisatos, A. P., Park, J. & McEuen, P. L., Fabrication of metallic electrodes with nanometer separation by electromigration. Appl. Phys. Lett. 75, 301 (1999).
- (7) Li, C. Z., Bogozi, A., Huang, W. & Tao, N. J., Fabrication of stable metallic nanowires with quantized conductance. Nanotechnology 10, 221-223 (1999).
- (8) Morpurgo, A. F., Marcus, C. M. & Robinson, D. B., Controlled fabrication of metallic electrodes with atomic separation. Appl. Phys. Lett. 74, 2084 (1999).
- (9) Agraït, N., Rodrigo, J. G. & Vieira, S., Conductance steps and quantization in atomic-size contacts. Phys. Rev. B 47, 12345-12348 (1993).
- (10) Pascual, J. I., et al., Quantum contact in gold nanostructures by scanning tunneling microscopy. Phys. Rev. Lett. 71, 1852-1855 (1993).
- (11) Brandbyge, M., et al., Quantized conductance in atom-sized wires between two metals. Phys. Rev. B 52, 8499 (1995).
- (12) Gai, Z., He Y., Yu, H. & Yang, W. S., Observation of conductance quantization of ballistic metallic point contacts at room temperature. Phys. Rev. B 53, 1042 (1996).
- (13) Yanson, A. I., Rubio Bollinger, G., van den Brom, H. E., Agraït, N. & van Ruitenbeek, J. M., Formation and manipulation of a metallic wire of single gold atoms. Nature 395, 783 (1998).
- (14) Krans, J. M., et al., One-atom point contacts. Phys. Rev. B 48, 14721-14724 (1993).
- (15) Olesen, L., et al., Quantised conductance in an atom-sized point contact. Phys. Rev. Lett. 72, 2251-2254 (1994).
- (16) Landauer, R., Spatial Variation of Currents and Fields Due to Localized Scatterers in Metallic Conduction. IBM J. Res. Dev. 1, 223 (1957).
- (17) Buettiker, M., Absence of backscattering in the quantum Hall effect in multiprobe conductors. Phys. Rev. B 38, 9375 (1988).
- (18) Imry, Y. & Landauer, R., Conductance viewed as transmission. Rev. Mod. Phys. 71, S306 (1999).
- (19) Delin, A. & Tosatti, E., Emerging magnetism in platinum nanowires. Surf. Sci. 566-568, 262-267 (2004).
- (20) Smogunov, A., Dal Corso, A. & Tosatti, E., Magnetic phenomena, spin-orbit effects, and Landauer conductance in Pt nanowire contacts: density-functional theory calculations. Phys. Rev. B 78, 014423 (2008).
- (21) Smogunov, A., Dal Corso, A., Delin, A., Weht, R. & Tosatti, E., Colossal Magnetic Anisotropy of Monatomic Free and Deposited Platinum Nanowires. Nature Nanotech. 3, 22 (2008).
- (22) Strigl, F., Espy, C., Bückle, M., Scheer, E. & Pietsch, T., Emerging magnetic order in platinum atomic contacts and chains. Nature Commun. 6, 6172 (2015).
- (23) Landman, U., Barnett, R. N., Cleveland, C. L. & Cheng, H.-P., Small is different. Int. J. Mod. Phys. B 6, 3623-3642 (1992).
- (24) Aviram, A. & Ratner, M. A., Molecular rectifiers. Chem. Phys. Lett. 29, 277-283 (1974).
- (25) Joachim, C., Gimzewski, J. K. & Aviram, A., Electronics using hybrid-molecular and mono-molecular devices. Nature 408, 541 (2000).
- (26) Tao, N. J., Electron transport in molecular junctions. Nature Nanotech. 1, 173 (2006).
- (27) Heath, J. R., Molecular electronics. Annu. Rev. Mater. Res. 39, 1-23 (2009).
- (28) Scott, G. D. & Natelson, D., Kondo resonance in molecular devices. ACS Nano 4, 3560 (2010).
- (29) Z̆utić, I., Fabian, J. & Das Sarma, S., Spintronics: fundamentals and applications. Rev. Mod. Phys. 76, 323 (2004).
- (30) Sanvito, S., Molecular spintronics. Chem. Soc. Rev. 40, 3336-3355 (2011).
- (31) Landman, U., Luedtke, W. D., Burnham, N. A. & Colton, R. J., Atomistic mechanisms and dynamics of adhesion, nanoindentation, and fracture. Science 248, 454 (1990).
- (32) Sutton, A. P. & Pethica, J. B., Inelastic flow processes in nanometre volumes of solids. J. Phys. Condens. Matter 2, 5317 (1990).
- (33) Gülseren, O., Ercolessi, F. & Tosatti, E., Noncrystalline Structures of Ultrathin Unsupported Nanowires. Phys. Rev. Lett. 80, 3775 (1998).
- (34) Nakamura, A., Brandbyge, M., Hansen, L. B. & Jacobsen, K. W., Density Functional Simulation of a Breaking Nanowire. Phys. Rev. Lett. 82, 1538 (1999).
- (35) Häkkinen, H., Barnett, R. N., Scherbakov, A. G. & Landman, U., Nanowire Gold Chains: Formation Mechanisms and Conductance. J. Phys. Chem. B 104, 9063 (2000).
- (36) Bahn, S. R. & Jacobsen, K. W., Chain formation of metal atoms. Phys. Rev. Lett. 87, 266101 (2001).
- (37) da Silva, E. Z., Novaes, F. D., da Silva, A. J. R. & Fazzio, A., Theoretical study of the formation, evolution, and breaking of gold nanowires. Phys. Rev. B 69, 115411 (2004).
- (38) Coura, P. Z., et al., On the Structural and Stability Features of Linear Atomic Suspended Chains Formed from Gold Nanowires Stretching. Nano Lett. 4, 1187 (2004).
- (39) Dednam, W., et al., Modeling contact formation between atomic-sized gold tips via molecular dynamics. J. Phys.: Conf. Ser. 574, 012045 (2015).
- (40) Tosatti, E., Nanowire formation at metal-metal contacts. Solid State Commun. 135, 610-617 (2005).
- (41) Torres, J. A., et al., The puzzling stability of monatomic gold wires. Surf. Sci. 426, L441 (1999).
- (42) Tosatti, E., Prestipino, P., Kostlmeier, S., Dal Corso, A. & Di Tolla, F. D., String Tension and Stability of Magic Tip-Suspended Nanowires. Science 291, 288 (2001).
- (43) Kondo, Y. & Takayanagi, K., Synthesis and Characterization of Helical Multi-Shell Gold Nanowires. Science, 289, 606 (2000).
- (44) Smit, R. H. M., Untiedt, C., Yanson, A. I. & van Ruitenbeek, J. M., Common Origin for Surface Reconstruction and the Formation of Chains of Metal Atoms. Phys. Rev. Lett. 87, 266102 (2001).
- (45) Yanson, A. I., Yanson, I. K. & van Ruitenbeek, J. M., Crossover from electronic to atomic shell structure in alkali metal nanowires. Phys. Rev. Lett. 87, 216805 (2001).
- (46) Urban, D. F., et al., Electronic shell effects and the stability of alkali nanowires. Sol. State Comm. 131, 609 (2004).
- (47) Kizuka, T., Atomic configuration and mechanical and electrical properties of stable gold wires of single-atom width. Phys. Rev. B 77, 155401 (2008).
- (48) Ercolessi, F., Parrinello, M. & Tosatti, E., Simulation of Gold in the Glue Model. Phil. Mag. A 58, 213-226 (1988).
- (49) Takeuchi, N., Chan, C. T. & Ho, K. M., Au(111): A theoretical study of the surface reconstruction and the surface electronic structure. Phys. Rev. B 40, 1565 (1989).
- (50) Lacroix, L.-M., Arenal, R. & Viau, G., Dynamic HAADF-STEM Observation of a Single-Atom Chain as the Transient State of Gold Ultrathin Nanowire Breakdown. J. Am. Chem. Soc. 136, 13075 (2014).
- (51) Scheer, E., et al., The signature of chemical valence in the electrical conduction through a single-atom contact. Nature 394, 154 (1998).
- (52) Brandbyge, M., Mozos, J-L., Ordejón, P., Taylor, J. & Stokbro, K., Density-functional method for nonequilibrium electron transport. Phys. Rev. B 65, 165401 (2002).
- (53) Mehrez, H., et al., I-V characteristics and differential conductance fluctuations of Au nanowires. Phys. Rev. B 65, 195419 (2002).
- (54) Palacios, J. J., Pérez-Jiménez, A. J., Louis, E., SanFabián, E. & Vergés, J. A., First-principles approach to electrical transport in atomic-scale nanostructures. Phys. Rev. B 66, 035322 (2002).
- (55) van Wees, B. J., et al., Quantized Conductance of Point Contacts in a Two-Dimensional Electron Gas. Phys. Rev. Lett. 60, 848-850 (1988).
- (56) Wharam, D. A., et al., One-dimensional transport and the quantisation of the ballistic resistance. J. Phys. C: Solid State Phys. 21, L209-L214 (1988).
- (57) Rubio, G., Agraït, N. & Vieira, S., Atomic-Sized Metallic Contacts: Mechanical Properties and Electronic Transport. Phys. Rev. Lett. 76, 2302 (1996).
- (58) Rubio-Bollinger, G., Bahn, S. R., Agraït, N., Jacobsen, K. W. & Vieira, S., Mechanical Properties and Formation Mechanisms of a Wire of Single Gold Atoms. Phys. Rev. Lett. 87, 026101 (2001).
- (59) Sorensen, M. R., Brandbyge, M. & Jacobsen, K. W., Mechanical deformation of atomic-scale metallic contacts: Structure and mechanisms. Phys. Rev. B 57, 3283 (1998).
- (60) Todorov, T. N. & Sutton, A. P., Force and conductance jumps in atomic-scale metallic contacts. Phys. Rev. B 54, R14234-R14237 (1996).
- (61) Calzolari, A., Marzari, N., Souza, I. & Buongiorno Nardelli, M., Ab initio transport properties of nanostructures from maximally localized Wannier functions. Phys. Rev. B 69, 035108 (2004).
- (62) Smogunov, A., Dal Corso, A. & Tosatti, E., Ballistic conductance of magnetic Co and Ni nanowires with ultrasoft pseudopotentials. Phys. Rev. B 70, 045417 (2004).
- (63) Choi, H. J. & Ihm, J., Ab initio pseudopotential method for the calculation of conductance in quantum wires. Phys. Rev. B 59, 2267 (1999).
- (64) Giannozzi, P., et al. Quantum Espresso: a modular and open-source software project for quantum simulations of materials. J. Phys.: Condens. Matter 21, 395502 (2009).
- (65) Untiedt, C., Dekker, D. M. T., Djukic, D. & van Ruitenbeek, J. M., Absence of magnetically induced fractional quantization in atomic contacts. Phys. Rev. B 69, 081401R (2004).
- (66) Sirvent, C., et al., Conductance step for a single-atom contact in the scanning tunneling microscope: Noble and transition metals. Phys. Rev. B 53, 16086 (1996).
- (67) Oshima, H. & Miyano, K., Spin-dependent conductance quantization in nickel point contacts. Appl. Phys. Lett. 73, 2203 (1998).
- (68) Ono, T., Ooka, Y., Miyajima, H. & Otani, Y., 2 to switching of quantum conductance associated with a change in nanoscale ferromagnetic domain structure. Appl. Phys. Lett. 75, 1622 (1999).
- (69) Bakker, D. J., Noat, Y., Yanson, A. I. & van Ruitenbeek, J. M., Effect of disorder on the conductance of a Cu atomic point contact. Phys. Rev. B 65, 235416 (2002).
- (70) Ludoph, B. & van Ruitenbeek, J. M., Conductance fluctuations as a tool for investigating the quantum modes in atomic-size metallic contacts. Phys. Rev. B 61, 2273 (2000).
- (71) Jacob, D., Fernandez-Rossier, J. & Palacios, J. J., Magnetic and orbital blocking in Ni nanocontacts. Phys. Rev. B 71, 220403R (2005).
- (72) Smogunov, A., Dal Corso, A. & Tosatti, E., Ballistic conductance and magnetism in short tip suspended Ni nanowires. Phys. Rev. B 73, 075418 (2006).
- (73) Bagrets, A., Papanikolaou, N. & Mertig, I., Magnetoresistance of atomic-sized contacts: an ab initio study. Phys. Rev. B 70, 064410 (2004).
- (74) Smogunov, A., Dal Corso, A. & Tosatti, E., Selective d-state conduction blocking in nickel nanocontacts. Surf. Sci. 507-510, 609-614 (2002).
- (75) Smogunov, A., Dal Corso, A. & Tosatti, E., Ballistic conductance of Ni nanowire with a magnetization reversal. Surf. Sci. 566-568, 390-395 (2004).
- (76) Autés, G., Barreteau, C., Desjonquéres, M. C., Spanjaard, D. & Viret, M. Giant orbital moments are responsible for the anisotropic magnetoresistance of atomic contacts. Europhys. Lett. 83, 17010 (2008).
- (77) Sokolov, A., Tsymbal, E. Y., Redepenning, J., Doudin, B., Quantized magnetoresistance in atomic-size contacts. Nature Nanotech. 2, 171 (2007).
- (78) Velev, J., Sabirianov, R. F., Jaswal, S. S., Tsymbal, E. Y., Ballistic anisotropic magnetoresistance. Phys. Rev. Lett. 94, 127203 (2005).
- (79) Smogunov, A., Dappe, Y. J., Symmetry-Derived Half-Metallicity in Atomic and Molecular Junctions. Nano Lett. 15, 3552 (2015).
- (80) Jacob, D., Fernández-Rossier, J. & Palacios, J. J., Emergence of half-metallicity in suspended NiO chains: Ab initio electronic structure and quantum transport calculations. Phys. Rev. B 74, 081402(R) (2006).
- (81) Delin, A. & Tosatti, E., Magnetic phenomena in 5d transition metal nanowires. Phys. Rev. B 68, 144434 (2003).
- (82) Gava, P., Dal Corso, A., Smogunov, A. & Tosatti, E., Magnetism-induced ballistic conductance changes in palladium nanocontacts. Eur. Phys. J. B75, 57 (2010).
- (83) Fernández-Rossier, J., Jacob, D., Untiedt, C. & Palacios, J. J., Transport in magnetically ordered Pt nanocontacts. Phys. Rev. B 72, 224418 (2005).
- (84) Smit, R. H. M., et al., Measurement of the conductance of a hydrogen molecule. Nature 419, 906 (2002).
- (85) Nielsen, S. K., et al., Conductance of single-atom platinum contacts: Voltage dependence of the conductance histogram. Phys. Rev. B 67, 245411 (2003).
- (86) Blanter, Ya. M. & Büttiker, M., Shot noise in mesoscopic conductors. Physics Rep. 336, 1-166 (2000).
- (87) van den Brom, H. E. & van Ruitenbeek, J. M., Quantum Suppression of Shot Noise in Atom-Size Metallic Contacts. Phys. Rev. Lett. 82, 1526 (1999).
- (88) Scheer, E., Joyez, P., Urbina, C. & Devoret, M. H., Conduction Channel Transmissions of Atomic-Size Aluminum Contacts. Phys. Rev. Lett. 78, 3535 (1997).
- (89) Chen, R., Matt, M., Pauly, F., Cuevas, J. C. & Natelson, D., Shot noise variation within ensembles of gold atomic break junctions at room temperature. J. Phys.: Condens. Matter 26, 474204 (2014).
- (90) Kumar, M., et al., Shot noise and magnetism of Pt atomic chains: Accumulation of points at the boundary. Phys. Rev. B 88, 245431 (2013).
- (91) Burtzlaff, A., Weismann, A., Brandbyge, M. & Berndt, R., Shot Noise as a Probe of Spin-Polarized Transport through Single Atoms. Phys. Rev. Lett. 114, 016602 (2015).
- (92) Hewson, A. The Kondo Problem to Heavy Fermions (Cambridge Univ. Press, 1993).
- (93) Madhavan, V., Chen, W., Jamneala, T., Crommie, M. F. & Wingreen, N. S., Tunneling into a single magnetic atom: spectroscopic evidence of the Kondo resonance. Science 280, 567-569 (1998).
- (94) Wahl, P., et al., Kondo Temperature of Magnetic Impurities at Surfaces. Phys. Rev. Lett. 93, 176603 (2004).
- (95) Manoharan, H. C., Lutz, C. P. & Eigler, D. M., Quantum mirages formed by coherent projection of electronic structure. Nature 403, 512 (2000).
- (96) Néel, N., et al., Conductance and Kondo Effect in a Controlled Single-Atom Contact. Phys. Rev. Lett. 98, 016801 (2007).
- (97) Vitali, L., et al., Kondo Effect in Single Atom Contacts: The Importance of the Atomic Geometry. Phys. Rev. Lett. 101, 216802 (2008).
- (98) Li, J., Schneider, W.-D., Berndt, R. & Delley, B., Kondo scattering observed at a single magnetic impurity. Phys. Rev. Lett. 80, 2893-2896 (1998).
- (99) Prüser, H., et al., Long-range Kondo signature of a single magnetic impurity. Nature Phys. 7, 203 (2011).
- (100) Calvo, M. R., et al., The Kondo effect in ferromagnetic atomic contacts. Nature 458, 1150 (2009).
- (101) Újsághy, O., Kroha, J., Szunyogh, L. & Zawadowski, A., Theory of the Fano resonance in the STM tunneling density of states due to a single Kondo impurity. Phys. Rev. Lett. 85, 2557-2560 (2000).
- (102) Park, J., et al., Coulomb blockade and the Kondo effect in single-atom transistors. Nature 417, 722-725 (2002).
- (103) Liang, W., Shores, M. P., Bockrath, M., Long, J. R. & Park, H., Kondo resonance in a single-molecule transistor. Nature 417, 725 (2002).
- (104) Parks, J. J., et al., Mechanical control of spin states in spin-1 molecules and the under screened Kondo effect. Science 328, 1370-1373 (2010).
- (105) Rakhmilevitch, D., Korytár, R., Bagrets, A., Evers, F. & Tal, O., Electron-Vibration Interaction in the Presence of a Switchable Kondo Resonance Realized in a Molecular Junction. Phys. Rev. Lett. 113, 236603 (2014).
- (106) Yu, L. H., et al., Inelastic Electron Tunneling via Molecular Vibrations in Single-Molecule Transistors. Phys. Rev. Lett. 93, 266802 (2004).
- (107) Parks, J. J., et al., Tuning the Kondo effect with a mechanically controllable break junction. Phys. Rev. Lett. 99, 026601 (2007).
- (108) Roch, N., Florens, S., Costi, T. A., Wernsdorfer, W. & Balestro, F., Observation of the underscreened Kondo effect in a molecular transistor. Phys. Rev. Lett. 103, 197202 (2009).
- (109) Osorio, E. A., et al., Electronic excitations of a single molecule contacted in a three-terminal configuration. Nano Lett 7, 3336-3342 (2007).
- (110) Frisenda, R., et al., Kondo Effect in a Neutral and Stable All Organic Radical Single Molecule Break Junction. Nano Lett. 15, 3109 (2015).
- (111) Wahl, P., et al., Kondo effect of molecular complexes at surfaces: Ligand control of the local spin coupling. Phys. Rev. Lett. 95, 166601 (2005).
- (112) Zhao, A., et al., Controlling the Kondo effect of an adsorbed magnetic ion through its chemical bonding. Science 309, 1542-1544 (2005).
- (113) Iancu, V., Deshpande, A. & Hla, S.-W., Manipulating Kondo temperature via single molecule switching. Nano Lett. 6, 820-823 (2006).
- (114) Komeda, T., et al., Observation and electric current control of a local spin in a single-molecule magnet. Nature Commun. 2, 217 (2011).
- (115) Mugarza, A., et al., Spin coupling and relaxation inside molecule-metal contacts. Nature Commun. 2, 490 (2011).
- (116) Minamitani, E., et al., Symmetry-Driven Novel Kondo Effect in a Molecule. Phys. Rev. Lett. 109, 086602 (2012).
- (117) Karan, S., et al., Shifting the Voltage Drop in Electron Transport Through a Single Molecule. Phys. Rev. Lett. 115, 016802 (2015).
- (118) Temirov, R., Lassise, A., Anders, F. B. & Tautz, F. S., Kondo effect by controlled cleavage of a single-molecule contact. Nanotechnology 19, 065401 (2008).
- (119) Müllegger, S., Rashidi, M., Fattinger, M. & Koch, R., Surface-supported hydrocarbon radicals show Kondo behavior. J. Phys. Chem. C 117, 5718-5721 (2013).
- (120) Zhang, Y.-H., et al., Temperature and magnetic field dependence of a Kondo system in the weak coupling regime. Nature Commun. 4, 2110 (2013).
- (121) Requist, R., et al., Kondo conductance across the smallest spin 1/2 radical molecule. Proc. Natl. Acad. Sci. USA 111, 69-74 (2014).
- (122) Xu, B. & Tao, N. J., Measurement of Single-Molecule Resistance by Repeated Formation of Molecular Junctions. Science 301, 1221 (2003).
- (123) Quek, S. Y., et al., Mechanically controlled binary conductance switching of a single-molecule junction. Nature Nanotech. 4, 230 (2009).
- (124) Aradhya, S. V. & Venkataraman, L., Single-molecule junctions beyond electronic transport. Nature Nanotech. 8, 399 (2013).
- (125) Haiss, W., et al., Redox State Dependence of Single Molecule Conductivity. J. Am. Chem. Soc. 125, 15294 (2003).
- (126) Sotthewes, K., Geskin, V., Heimbuch, R., Kumar, A. & Zandvliet, H. J. W., Research Update: Molecular electronics: The single-molecule switch and transistor. APL Materials 2, 010701 (2014).
- (127) Lucignano, P., Mazzarello, R., Smogunov, A., Fabrizio, M. & Tosatti, E., Kondo conductance in an atomic nanocontact from first principles. Nature Mat. 8, 563-567 (2009).
- (128) Bulla, R., Costi, T. A. & Pruschke, T., Numerical renormalization group method for quantum impurity systems. Rev. Mod. Phys. 80, 395-450 (2008).
- (129) Z̆itko, R. & Pruschke, T., Energy resolution and discretization artifacts in the numeric renormalization group. Phys. Rev. B 79, 085106 (2009).
- (130) Baruselli, P. P., Requist, R., Smogunov, A., Fabrizio, M. & Tosatti, E., Co adatoms on Cu surfaces: ballistic conductance and Kondo temperature. Phys. Rev. B 92, 045119 (2015).
- (131) Baruselli, P. P., Smogunov, A., Fabrizio, M. & Tosatti, E., Kondo effect of magnetic impurities in nanotubes. Phys. Rev. Lett. 108, 206807 (2012).
- (132) Dias da Silva, L. G. G. V., Tiago, M. L., Ulloa, S. E., Reboredo, F. A. & Dagotto, E. Many-body electronic structure and Kondo properties of cobalt-porphyrin molecules. Phys Rev B 80, 155443 (2009).
- (133) Cornaglia, P. S., Roura Bas, P., Aligia, A. A. & Balseiro, C. A., Quantum transport through a stretched spin-1 molecule. Europhys. Lett. 93, 47005 (2010).
- (134) Jacob, D., Haule, K. & Kotliar, G., Kondo Effect and Conductance of Nanocontacts with Magnetic Impurities. Phys. Rev. Lett. 103, 016803 (2009).
- (135) Costi, T. A., et al., Finding the right spin model for iron impurities in gold and silver. Phys. Rev. Lett. 102, 056802 (2009).
- (136) Surer, B., et al., Multiorbital Kondo physics of Co in Cu hosts. Phys. Rev. B 85, 085114 (2012).
- (137) Jacob, D., Soriano, M. & Palacios, J. J., Kondo effect and spin quenching in high-spin molecules on metal substrates. Phys. Rev. B 88, 134417 (2013).
- (138) Nozières, P., A “fermi-liquid” description of the Kondo model at low temperatures. J. Low Temp. Phys. 17, 31 (1974).
- (139) Nozières, P. & Blandin, A., Kondo effect in real metals. J. Phys. (Paris) 41, 193 (1980).
- (140) Koller, W., Hewson, A. C. & Meyer, D., Singular dynamics of underscreened magnetic impurity models. Phys. Rev. B 72, 045117 (2005).
- (141) Mehta, P., Andrei, N., Coleman, P., Borda, L. & Zarand, G., Regular and singular Fermi-liquid fixed points in quantum impurity models. Phys. Rev. B 72, 014430 (2005).
- (142) Anderson, P. W., A poor man’s derivation of scaling laws for the Kondo problem. J. Phys. C.: Solid State Phys. 3, 2436 (1970).
- (143) Baruselli, P. P, Requist, R., Fabrizio, M. & Tosatti, E., Ferromagnetic Kondo Effect in a Triple Quantum Dot System. Phys. Rev. Lett. 111, 047201 (2013).
- (144) Gentile, P., De Leo, L., Fabrizio, M. & Tosatti, E., Lack of Kondo screening at nanocontacts of nearly magnetic metals. Eur. Phys. Lett. 87, 27014 (2009).
- (145) Kuzmenko, T., Kikoin, K. & Avishai, Y., Tunneling through triple quantum dots with mirror symmetry. Phys. Rev. B 73, 235310 (2006).
- (146) Mitchell, A. K., Jarrold, T. F., Galpin, M. R. & Logan, D. E., Local Moment Formation and Kondo Screening in Impurity Trimers. J. Phys. Chem. B 117, 12777 (2013).
- (147) Andrade, J. A., García, D. J. & Cornaglia, P. S., Ferromagnetic and underscreened Kondo behavior in quantum dot arrays. Phys. Rev. B 92, 165416 (2015).
- (148) Metzger, R. M., Unimolecular electrical rectifiers. Chem. Rev. 103, 3803 (2003).
- (149) Elbing, M., et al., A single-molecule diode. Proc. Natl. Acad. Sci. USA 102, 8815-8820 (2005).
- (150) Díez-Pérez, I., et al., Rectification and stability of a single molecular diode with controlled orientation. Nature Chem. 1, 635 (2009).
- (151) Batra, A., et al., Tuning Rectification in Single-Molecular Diodes. Nano Lett. 13, 6233-6237 (2013).
- (152) Park, H., et al., Nanomechanical oscillations in a single-C transistor. Nature 407, 57 (2000).
- (153) Roch, N., Florens, S., Bouchiat, V., Wernsdorfer, W. & Balestro, F., Quantum phase transition in a single-molecule quantum dot. Nature 453, 633 (2008).
- (154) Song, H., et al., Observation of molecular orbital gating. Nature 462, 1039 (2009).
- (155) Martínez-Blanco, J., et al., Gating a single-molecule transistor with individual atoms. Nature Phys. 11, 640-644 (2015).
- (156) Sivkov, I. N., Brovko, O. O., Bazhanov, D. I. & Stepanyuk, V. S., Emergence of high spin polarization of conductance in atomic-size Co-Au contacts. Phys. Rev. B 89, 075436 (2014).
- (157) Pati, R., Senapati, L., Ajayan, P. M. & Nayak, S. K., First-principles calculations of spin-polarized electron transport in a molecular wire: Molecular spin valve. Phys. Rev. B 68, 100407R (2003).
- (158) Rocha, A. R., et al., Towards molecular spintronics. Nature 4, 335 (2005).
- (159) Schmaus, S., et al., Giant magnetoresistance through a single molecule. Nature Nanotech. 6, 185 (2011).
- (160) Tao, L. L., Liang, S. H., Liu, D. P. & Han, X. F., Large magnetoresistance of paracyclophane-based molecular tunnel junctions: A first-principles study. J. Appl. Phys. 114, 213906 (2013).
- (161) Zu, F., et al., Nearly perfect spin filter, spin valve and negative differential resistance effects in a Fe-based single-molecule junction. Sci. Rep. 4, 4838 (2013).
- (162) Vardimon, R., Klionsky, M. & Tal, O., Indication of Complete Spin Filtering in Atomic-Scale Nickel Oxide. Nano Lett. 15, 3894 (2015).
Work in Trieste partly sponsored by ERC Advanced Grant 320796 – MODPHYSFRICT.
Competing financial interests
The authors declare no competing financial interests.